General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 12.4 g/cm³ Show Material materials with Density of 12.4 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -190.0 °C | 405 GPa Show Material materials with Elastic modulus of 405 GPa |

20.0 °C | 380 - 386 GPa Show Material materials with Elastic modulus of 380 - 386 GPa | |

200.0 °C | 368 GPa Show Material materials with Elastic modulus of 368 GPa | |

400.0 °C | 346 GPa Show Material materials with Elastic modulus of 346 GPa | |

500.0 °C | 336 GPa Show Material materials with Elastic modulus of 336 GPa | |

600.0 °C | 325 GPa Show Material materials with Elastic modulus of 325 GPa | |

700.0 °C | 315 GPa Show Material materials with Elastic modulus of 315 GPa | |

800.0 °C | 304 GPa Show Material materials with Elastic modulus of 304 GPa | |

900.0 °C | 291 GPa Show Material materials with Elastic modulus of 291 GPa | |

Elongation | 20.0 °C | 9 % Show Material materials with Elongation of 9 % |

Hardness, Vickers | 20.0 °C | 120 - 410 [-] Show Material materials with Hardness, Vickers of 120 - 410 [-] |

Poisson's ratio | 20.0 °C | 0.26 [-] Show Material materials with Poisson's ratio of 0.26 [-] |

Shear modulus | 20.0 °C | 150 - 153 GPa Show Material materials with Shear modulus of 150 - 153 GPa |

Tensile strength | -196.0 °C | 879 MPa Show Material materials with Tensile strength of 879 MPa |

20.0 °C | 690 - 800 MPa Show Material materials with Tensile strength of 690 - 800 MPa | |

25.0 °C | 720 MPa Show Material materials with Tensile strength of 720 MPa | |

250.0 °C | 622 MPa Show Material materials with Tensile strength of 622 MPa | |

500.0 °C | 343 MPa Show Material materials with Tensile strength of 343 MPa | |

750.0 °C | 119 MPa Show Material materials with Tensile strength of 119 MPa | |

1000.0 °C | 86 MPa Show Material materials with Tensile strength of 86 MPa | |

Unlock all property charts | ||

Yield strength | -196.0 °C | 65 MPa Show Material materials with Yield strength of 65 MPa |

20.0 °C | 68 MPa Show Material materials with Yield strength of 68 MPa | |

25.0 °C | 50 MPa Show Material materials with Yield strength of 50 MPa | |

250.0 °C | 76 MPa Show Material materials with Yield strength of 76 MPa | |

500.0 °C | 59 MPa Show Material materials with Yield strength of 59 MPa | |

750.0 °C | 24 MPa Show Material materials with Yield strength of 24 MPa | |

1000.0 °C | 25 MPa Show Material materials with Yield strength of 25 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2 | -196.0 °C | 94 MPa Show Material materials with Yield strength Rp0.2 of 94 MPa |

20.0 °C | 69 - 270 MPa Show Material materials with Yield strength Rp0.2 of 69 - 270 MPa | |

25.0 °C | 68 MPa Show Material materials with Yield strength Rp0.2 of 68 MPa | |

250.0 °C | 97 MPa Show Material materials with Yield strength Rp0.2 of 97 MPa | |

500.0 °C | 77 MPa Show Material materials with Yield strength Rp0.2 of 77 MPa | |

750.0 °C | 41 MPa Show Material materials with Yield strength Rp0.2 of 41 MPa | |

1000.0 °C | 35 MPa Show Material materials with Yield strength Rp0.2 of 35 MPa | |

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 50.0 °C | 8E-6 1/K Show Material materials with Coefficient of thermal expansion of 8E-6 1/K | |

100.0 °C | 8.5E-6 1/K Show Material materials with Coefficient of thermal expansion of 8.5E-6 1/K | ||

200.0 °C | 9E-6 1/K Show Material materials with Coefficient of thermal expansion of 9E-6 1/K | ||

300.0 °C | 9.3E-6 1/K Show Material materials with Coefficient of thermal expansion of 9.3E-6 1/K | ||

400.0 °C | 9.6E-6 1/K Show Material materials with Coefficient of thermal expansion of 9.6E-6 1/K | ||

500.0 °C | 9.8E-6 1/K Show Material materials with Coefficient of thermal expansion of 9.8E-6 1/K | ||

600.0 °C | 1E-5 1/K Show Material materials with Coefficient of thermal expansion of 1E-5 1/K | ||

700.0 °C | 1.01E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.01E-5 1/K | ||

800.0 °C | 1.03E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.03E-5 1/K | ||

900.0 °C | 1.05E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 1/K | ||

1000.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | ||

1100.0 °C | 1.1E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.1E-5 1/K | ||

1200.0 °C | 1.13E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.13E-5 1/K | ||

1300.0 °C | 1.15E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.15E-5 1/K | ||

1400.0 °C | 1.18E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.18E-5 1/K | ||

1500.0 °C | 1.21E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.21E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1963 °C Show Material materials with Melting point of 1963 °C | Typical for Rhodium | |

Specific heat capacity | 23.0 °C | 254 J/(kg·K) Show Material materials with Specific heat capacity of 254 J/(kg·K) | Typical for Rhodium |

Thermal conductivity | -173.0 °C | 185 W/(m·K) Show Material materials with Thermal conductivity of 185 W/(m·K) | |

-73.0 °C | 156 W/(m·K) Show Material materials with Thermal conductivity of 156 W/(m·K) | ||

20.0 °C | 88 W/(m·K) Show Material materials with Thermal conductivity of 88 W/(m·K) | ||

127.0 °C | 145 W/(m·K) Show Material materials with Thermal conductivity of 145 W/(m·K) | ||

327.0 °C | 135 W/(m·K) Show Material materials with Thermal conductivity of 135 W/(m·K) | ||

527.0 °C | 126 W/(m·K) Show Material materials with Thermal conductivity of 126 W/(m·K) | ||

727.0 °C | 121 W/(m·K) Show Material materials with Thermal conductivity of 121 W/(m·K) | ||

927.0 °C | 118 W/(m·K) Show Material materials with Thermal conductivity of 118 W/(m·K) | ||

1127.0 °C | 115 W/(m·K) Show Material materials with Thermal conductivity of 115 W/(m·K) | ||

1327.0 °C | 109 W/(m·K) Show Material materials with Thermal conductivity of 109 W/(m·K) | ||

1527.0 °C | 106 W/(m·K) Show Material materials with Thermal conductivity of 106 W/(m·K) | ||

1727.0 °C | 104 W/(m·K) Show Material materials with Thermal conductivity of 104 W/(m·K) | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical conductivity | 20.0 °C | 2.33E+7 S/m Show Material materials with Electrical conductivity of 2.33E+7 S/m |

Electrical resistivity | 20.0 °C | 4.3E-8 Ω·m Show Material materials with Electrical resistivity of 4.3E-8 Ω·m |

Chemical properties

Property | Value |
---|---|

Rhodium | 99.9 % Show Material materials with Rhodium of 99.9 % |